Full Text - Mineralogical Society of America
Volume 84, pages 207-2/0,
A moganite-type phase in the silica analog phosphorus oxynitride
AND ROGER MARCHAND
ILaboratoire de Physico-Chimie des Materiaux, Centre National de la Recherche Scientifique, I place Aristide Briand, 92195 Meudon cedex, France
2 LaboratOlre des Verres et Ceramiques, UMR CNRS 6512, Universite de Rennes I, Campus de Beaulieu, Bat. 10, Avenue du General Leclerc, 35042
A new polymorph of phosphorus oxynitride (PON) a silica analog has been recovered at ambient
pressure by quenching after a treatment at 850°C under a pressure of 2.5 GPa using cristobalite- or
quartz-type phases as starting materials. This PON polymorph is a thermodynamically
w~th its own stability field in a P-T diagram. The structure of this PON phase was refined by the
RIetveld method from an X-ray powder diffractogram. It is isostructural with "moganite" (Si02).
The discovery of this PON polymorph should stimulate a renewed interest in the occurrence of this
phase in the silica system, because "moganite" may have a small but defined P-T stability field.
These results confirm the structure of "moganite" as a new structure-type in AX2 compounds.
The natural abundance, geological and geophysical importance, and technological properties of silica make it one of the
most thoroughly studied compounds. Its polymorphism is very
complex (Heaney et al. 1994), as the numerous crystalline and
amorphous phases are built of corner-sharing Si04 tetrahedra
(below about 10 GPa). These tetrahedra can be linked in many
different ways and, in addition, are able to tilt easily under the
influence of temperature and/or pressure. Although silica polymorphism has been studied extensively, the stability of the
phases at atmospheric or low pressures (below I GPa) is not
yet established clearly. At atmospheric pressure, cristobalite is
the stable high-temperature phase; quartz is a lower-temperature higher-pressure phase, which is stable at room temperature. Both quartz and cristobalite undergo displacive CI.-~transitions. Whether ~-quartz transforms directly to cristobalite, or
whether there is a stable phase field for tridymite, an intermediate phase between quartz and cristobalite has been disputed
(Navrotsky 1994). The calculated cristobalite-tridymite phase
boundary does not agree well with reversal experiments of
Swamy et al. (1994). It is not yet clear whether tridymite has a
stability field in the pure SiOz system; furthermore, several
modifications of tridymite exist. A new silica polymorph was
found in some of the ignimbrite flows of the Mogan formation
of Gran Canaria and was described by Harke et al. (1976). This
polymorph of silica has not yet been recognized by the l.M.A.
as a mineral species and will be referred to herein as "moganite."
This polymorph occurs as microcrystalline fillings of cavities,
fissures, and cooling cracks in natural formations. The presence of 2-3 wt% water was detected in natural samples but this
water is not essential to the structure. Moganite persists at temperatures at which the samples have already lost their entire
content of water. This novel silica polymorph was later shown
by Heaney and Post (1992) to be widespread in microcrystalline quartz varieties, and its presence may explain differences
in phase boundary determinations using natural samples of
quartz. Moganite may be a stable phase of silica; however, it
has not yet been synthesized experimentally nor has its P-Tfield
of thermodynamic stability been determined.
Many compounds have structures built of corner-sharing
tetrahedra and display several phases isostructural with those
observed among the silica polymorphs. Ge04 tetrahedra are
larger than the Si04 tetrahedra, and the pressure-induced transitions in Ge02 are lowered with respect to those in silica and
thus the stability fields of the lower pressure phases are reduced.
The stable phases at atmospheric pressure are the quartz-type
at high temperature and the rutile-type at low temperature; the
latter phase is built of octahedra like those found in stishovite,
which is found above 9 GPa. Several AB04 (A = B, AI, Ga, and
B = As, P) silica analogs crystallize in the cristobalite- or quartztype structures as described by O'Keefe and Hyde (1976). For
example, BP04 and BAs04 crystallize in cristobalite-type structures at atmospheric pressure and transform under higher pressure to the quartz-type structures (Fukunaga and Yamaoka 1979).
However, the different sizes of the A04 and B04 tetrahedra make
comparisons with silica difficult.
Other silica analogs exist, in which there are only one cation and two anions of approximately the same size. Phosphorus oxynitride, PON, is one such example. At atmospheric pressure, Boubkir et al. (1989) showed by neutron diffraction that
PON adopts a slightly distorted variant of the structure of ~cristobalite, the high-temperature polymorph of silica. The structure belongs to the space group P 4, Z = 4, with a = 4.6266(1)
*E-mail: [email protected]
A and c = 7.0037(3) A. The atomic positions are displaced by
only ~ few standard deviations with respect to the positions in
the 14 2d structure type found in silica. The oxygen and nitrogen atoms are completely disordered over 4h sites. At 4.5 GPa
and 750°C, Miller et al. (1981) observed that cristobalite-type
PON transforms to a quartz-type phase with a trigonal unit cell.
The structure of this phase was refined by Leger et al. (1998)
by neutron diffraction at atmospheric conditions [P3221, Z = 3;
a = 4.757(4) A, c = 5.2460(2) A).The oxygen and nitrogen atoms are disordered over the available anion sites. The structure
ET AL.: MOGANITE-TYPE
PHASE IN PHOSPHOROUS
is very close to that of a-quartz (P3z2l, Z = 3; a = 4.913 A and c =
5.405 A) and the fractional atomic coordinates differ by less than
The structures of these PON phases and those of the silica polymorphs are built ofAX4 tetrahedra. Because p5+ is smaller than
Si4+,the P(O,N)4 tetrahedra are smaller than the Si04 tetrahedra in
SiOz, and higher pressures are required than for SiOz to induce
phase changes in PON. The quartz-type phase of PON is effectively prepared only at high pressure and not at atmospheric pressure. In PON, the phase transformations
are displaced toward
higher pressures relative to those in SiOzleading to extended fields
of stability facilitating the study of the lower pressure phases.
In this Letter, we report the occurrence of a new phase in PON
obtained by high-pressure, high-temperature
treatment. This is a
stable phase because it can be obtained either from the cristobaliteor the quartz-type phases; it has a structure that is very similar to
moganite. The pressure-induced
in PON is thus
very similar to that of SiOz and could shed light on the polymorphism of SiOz and help in identifying potential thermodynamically stable phases at lower pressures.
EXPERIMENTAL PROCEDURE AND RESULTS
Cristobalite-type PON was prepared as described previously
by Boubkir et al. (1989). No trace of any other crystalline phase
was detected. Transformation ofPON from the cristobalite- to the
quartz-type phase occurred at 4.5 OPa and 750°C, as reported
previously by Miller et al. (1981) using the same techniques as
described below. Cristobalite- and quartz-type PON samples were
used as the starting materials for the high-pressure synthesis of
Samples of 10-50 mg were placed in crucibles made of platinum or in gold tubes closed by end disks; these crucibles were
placed in boron nitride tubes surrounded by a graphite heater and
pyrophyllite jackets. They were subjected to high-pressure, hightemperature treatments in a belt type apparatus as described by
Boire et al. (1991). The pressure was first increased at room temperature and was determined from a previous calibration curve.
The temperature was then increased at constant load pressure, and
the temperature at the center of the cell was monitored with a
chromel-alumel thermocouple. The vertical temperature gradients
in the high-pressure cell of about 60 °C/mm were measured with
a second off-center thermocouple. In a single run, several samples
placed at different heights along the vertical axis thus could be
subjected to the same pressure but different temperatures. After
temperature quenching followed by slow decompression, the
samples were recovered and analyzed using an X-ray diffractometer (CuKa radiation) equipped with a curved graphite diffracted-beam monochromator.
Treatment of the cristobalite phase of PON at 2.5 OPa and 850
°C for one hour yielded a new phase that was isostructural with
moganite. This recovered sample consisted almost entirely of the
pure moganite-type phase, with only 1.6% of the quartz-type phase
and 1.1% of the cristobalite-type phase (Fig. 1). The temperature
gradient in the high-pressure cell proved to be sufficient to obtain
different transformation yields according to the exact temperature, which can explain the presence of quartz- and cristobalitetype phases in the recovered samples. At 800°C, the conversion
of cristobalite- to moganite-type PON was not complete, and about
11111 t 111111111t 1111111111II III II 11111111111111
II I I
I I III
I I I 1111 II II
I I I
I II 1111
1111 I I
FIGURE I. Experimental (-) and calculated (solid line) X-ray (CuKa
radiation) powder diffraction profile from the Rietveld refinement of
(M) PON. Intensity is in arbitrary units and the difference
profile is shown on the same scale; vertical bars indicate all possible Bragg
(Q and C, respectively)
reflections. Some quartz- and cristobalite-type
PON was detected (1.6 and 1.1 %, respectively);
trace gold from the
crucible was also detected on the surface sample.
6% of the former remained after one hour. In comparison, 30% of
the cristobalite-type PON remained after one hour at 775°C. At
700°C, no conversion was observed. Complete conversion of the
cristobalite- to the moganite-type phase was obtained at 1.8 OPa
and 900°C. Starting from the quartz-type phase, the resultant
moganite-type phase was mixed with 2% cristobalite-type phase
at 2.5 OPa and 835°C. At 750 °C, little transformation was obtained, and the recovered sample consisted of 80% untransformed
quartz-type and 20% moganite-type phases.
These experiments reveal that moganite-type PON was obtained at 2.5 OPa and 850°C starting from either the cristobaliteor the quartz-type phases. Moganite-type PON is thus a thermodynamically stable phase with its own field stability in the P-T
The X-ray powder diffractogram of this new PON phase is
shown in Figure 1. It is very similar to the diffraction pattern of
moganite obtained by Miehe and Oraetsch (1992). However, the
diffraction lines from PON are much sharper than those reported
for moganite and a crystallite size on the order of 70 nm was deduced from their widths. This was in agreement with the visual
examination of the sample. After the high-pressure synthesis, the
sample was a sintered powder that appeared grayish; after grinding, translucent grains (1-10 ).lmin size with no particular shapes)
TABLE 1. Cell parameters
for the moganite-type
of PON and
of Miehe and Graetsch
ET AL.: MOGANITE-TYPE
TABLE 2. Atomic positions in the moganite-type
PHASE IN PHOSPHOROUS
phases of PON* and Si02
(0, N) or O.
Notes: /2/a, Z = 12; A = P or Si, X =
(A') = 3.86(3).
tPositions of Miehe and Graetsch (1992).
composed of aggregated smaller particles were observed.
Structurerefinements wereperformed using a moganite structural model (see Tables I and 2) with the Fullprof program
(Rodiguez-Carvajal, unpublished). Four phases were included in
the refinement: the cristobalite-, quartz-, and moganite-type PON
phases and gold metal (trace from the crucible); 97% of the investigated sample was in the moganite-type phase. For the latter, the
scale factor, the line shape parameters, the lattice constants, the
atomic positions and the overall atomic displacement parameter
were refined. For the cristobalite- and quartz-type phases, only
the scale factors were refined; for gold, the scale factor, the lineshape parameters, the lattice constant, and the overall atomic displacement parameter were refined. The refinement converged rapidly and it was not necessary to impose any constraints in contrast
to the study of Miehe and Graetsch (1992) in which it was necessary to fix the position of 1 0 atom (02) based on the results of
distance least-squares calculations. The Bragg agreement factor
was 4.8% ; the unweighted profile and weighted profile agreement factors were 14.9 and 13.3%, respectively.
The structure of moganite-type PON is monoclinic, I2/a, Z =
12, a = 8.5173(5) A, b = 4.7453(3) A, c = 10.3990(6) A, and p =
90.00(1)°. The oxygen and nitrogen atoms were assumed to be
disordered over the available anion sites as in the quartz-type phase
of PON, and their occupation factor was set to 0.5. Atoms are on
the general 8f positions except for P(I) which is on 4e positions
(1/4, y, 0) . The atomic positions in moganite-type PON are in-
TABLE 3. Selected bond distances (A) in moganite-type
PON and Si02
'Values of Miehe and Graetsch (1992) with 02 fixed based on results of
distance least-squares calculations.
t'j, - x, y, oz.
§'j, + x, - y, z.
II-x, 'j, + y, 'j, - z.
deed very close to those in moganite (Table 2). The refined fractional atomic coordinates of phosphorus and (O,N) differ from
the respective values of silicon and oxygen in silica by less than
0.020 and in most cases by less than 0.008. The A-X distances in
the AX. tetrahedra are given in Table 3; they are typically 0.06 A
less in PON than in Si02 and range from 1.527(9) to 1.575(6) A
in PON and 1.596 to 1.636 A in SiO, (average 1.554 and 1.615 A,
The structure of moganite was described by Miehe and Graetsch
(1992). It is based on alternating slabs of left- and right-handed
quartz. In addition to the six- and eight-membered rings, the structure contains four-membered rings of SiO. tetrahedra, which form
chains in the direction of the x axis. Chains of this type are not
known in other silica polymorphs, but they do occur in aluminosilicates.
The occurrence of the moganite-type phase in PON confirms
the close structural similarities between PON and SiO,. The atomic
positions observed in the PON and SiO, polymorphs are always
very close in each structure-type adopted. The three phases known
in PON under atmospheric conditions or at high pressure have the
same structures as three phases of silica obtained at atmospheric
pressure, although there is a slight distortion in the case of the.
Two of these PON polymorphs cannot be prepared at atmospheric pressure but only under high pressure, which shows that
the stability fields of the lower pressure phases are extended toward higher pressures in PON compared to Si02. The moganitetype phase of PON is found between the cristobalite- and quartztype phases upon increasing pressure at high temperature: it is a
phase with respect to the
conditions, the molar volumes for the
cristobalite-, moganite- and quartz-type phases of PON are 22.58,
21.05, and 20.64 cm3, respectively. In silica, the molar volumes
of the corresponding phases (25.93, 22.97, and 22.69 cm3) follow
the same trend, and the stability field of moganite should lie in the
same relative place, between cristobalite and quartz. This is precisely where tridymite is found, the thermodynamic stability of
which has not been confirmed. However, the relative volume difference between the moganite- and quartz-type phases is larger in
PON (2.0%) than in silica (1.2%). This difference could explain
why the moganite-type phase can be readily isolated in PON
whereas in silica, it is always found mixed with microcrystalline
ET AL.: MOGANITE-TYPE
quartz. Moganite could be the thermodynamically
phase under temperature and pressure conditions close to the
boundary. However, the question of the stability
ofmoganite has not been answered, as stated by Navrotsky (1994).
Upon heating a moganite sample at 900°C, the beginning of a
to disordered cristobalite was detected by Miehe and Graetsch (1992). No tridymite phase was
observed, although this transformation occurs in the temperature
range where tridymite is generally encountered. This confirms that
the stability field of moganite could occupy part of that currently
attributed to tridymite. Moganite has not been obtained via direct
The smaller size of the P(O,N)4 tetrahedron relative to that of
Si04 widens the pressure fields of stability for the lower pressure
phases, which allowed for the discovery of the P- T stability field
of the moganite-type phase of PON. The stability field of moganite
itself may be small and partially occupy that attributed to tridymite.
In addition, the present results confirm the moganite-type structure as a new structure-type in AX2 compounds.
Boire, P., Chateau. C. Leger. J.M., Suryanarayanan, R., Gorochov, 0., and Quitmann,
C. (1991) Superconducting properties of Yba2Cu,0, treated under high pressure
PHASE IN PHOSPHOROUS
and high temperature. Superconductor
Science and Technology, 4,137-142.
Boubkir, L., Marchand, R., Laurent, Y, Bacher, P., and Roult, G. (1989) Preparation and
time-of-flight neutron diffraction study of the cristobalite-type
oxynitride. Annales de Chimie, 14,475-481.
FlUrke, O.w., Jones, J.B., and Schmincke, H.U. (1976) A new microcrystalline
from Gran Can aria. Zeitschrift fUr Kristallographie,
Fukunaga, 0. and Yamaoka, S. (1979) Phase transformation in ABO, type compounds
under high pressure. Physics and Chemistry of Minerals, 5,167-177.
Heaney. P.J. and Post, J.E. (1992) The widespread distribution of a novel silica polymorph in microcrystalline
quartz varieties. Science, 255, 441-443.
Heaney, P.J., Prewitt, CT., and Gibbs, G.Y. (1994) Silica: physical behavior, geochemistry and materials applications. In Mineralogical Society of America Reviews in
Mineralogy, 29, 606 p.
Leger, J.M., Haines, J., de Oliveira, L.S.. Chateau, C, LeSauze, A., Marchand, R., and
Hull, S. (1998) Crystal structure and high pressure behaviour of the quartz-type
phase of phosphorus oxynitride PON. Journal of Physics and Chemistry of Solids,
Miehe, G. and Graetsch, H. (1992) Crystal structure of moganite : a new structure type
for silica. European Journal of Mineralogy, 4,693-706.
Miller, T.N., Vitola,A.A., Vilk, Y.N., Bondars, B.I., and Davidenko, Y.M. (1981) New
modification of phosphorus oxynitride. Izvestia Academy Nauk SSR, Serya Chimia,
Navrotsky, A. (1994) Thermochemistry
of crystalline and amorphous silica. In Mineralogical Society of America Reviews in Mineralogy, 29, 309-329.
O'Keefe, M. and Hyde, B.G. (1976) Cristobalites and topologically-related
MANUSCRIPT RECEIVED JUNE 15, 1998
MANUSCRIPT ACCEPTED OCTOBER I, 1998
PAPER HANDLED BY WILLIAM A. BASSETT